- Nano Express
- Open Access
Optical Properties of Silicon Nanowires Fabricated by Environment-Friendly Chemistry
© The Author(s). 2016
- Received: 20 April 2016
- Accepted: 28 July 2016
- Published: 9 August 2016
Silicon nanowires (SiNWs) were fabricated by metal-assisted chemical etching (MACE) where hydrofluoric acid (HF), which is typically used in this method, was changed into ammonium fluoride (NH4F). The structure and optical properties of the obtained SiNWs were investigated in details. The length of the SiNW arrays is about 2 μm for 5 min of etching, and the mean diameter of the SiNWs is between 50 and 200 nm. The formed SiNWs demonstrate a strong decrease of the total reflectance near 5–15 % in the spectral region λ < 1 μm in comparison to crystalline silicon (c-Si) substrate. The interband photoluminescence (PL) and Raman scattering intensities increase strongly for SiNWs in comparison with the corresponding values of the c-Si substrate. These effects can be interpreted as an increase of the excitation intensity of SiNWs due to the strong light scattering and the partial light localization in an inhomogeneous optical medium. Along with the interband PL was also detected the PL of SiNWs in the spectral region of 500–1100 nm with a maximum at 750 nm, which can be explained by the radiative recombination of excitons in small Si nanocrystals at nanowire sidewalls in terms of a quantum confinement model. So SiNWs, which are fabricated by environment-friendly chemistry, have a great potential for use in photovoltaic and photonics applications.
- Silicon nanowires
- Environment-friendly chemistry
- Total reflectance
- Raman scattering
In the last years, silicon nanowires (SiNWs) are of great interest because of their potential applications in micro- and optoelectronics [1, 2], photonics , photovoltaics [4, 5], and sensorics [6–8]. Initially, SiNWs were obtained by vapor-liquid-solid method with the help of a noble metal (mostly gold, Au) which was first proposed by Wagner and Ellis in 1964 . An alternative method was metal-assisted chemical etching (MACE) by which initially it was believed that the porous silicon (PSi) was obtained [10, 11]. MACE is based on the anisotropic etching of crystalline silicon (c-Si) in aqueous solutions which are usually based on hydrofluoric acid (HF) [10–15]. The reaction is catalyzed by metal nanoparticles such as Au [10, 12], Ag , or Pt [10, 11] at the substrate surface, and the oxidizing agents are H2O2 [10–13], KMnO4 , or Fe(NO3)3 . It has been shown that SiNWs, which were obtained by MACE, are found to possess such remarkable optical properties as visible photoluminescence (PL) , extremely low total reflection [17, 18], enhancement of Raman scattering [17, 19–21], coherent anti-Stokes light scattering , interband PL [17, 19–21] and efficiency of generation of third harmonics  in comparison with the corresponding intensities for c-Si, and sensitivity of visible PL to molecular surroundings . However, HF is rather toxic and may also result in hypocalcemia and hypomagnesemia . Therefore, there is great interest in the study of possible modifications of the MACE method by using environment-friendly chemistry.
Ammonium fluoride (NH4F) has long been used for SiO2 dissolution. It has been shown that the SiO2 etch rate in aqueous NH4F solutions depends on the pH and on the NH4F concentration . Then, aqueous NH4F solution was proposed as an alternative of HF in the electrochemical method of obtaining PSi films [27–29]. Furthermore, the microstructure properties of the fabricated PSi have shown a strong dependency from the pH of the electrolyte. A pebble-like surface structure was formed during anodization at pH 4.5, while nanoporous Si layers were formed at lower pH . Also, the usage of NH4F as the etchant allows it to survive the aluminum contact during the etching process, because the aluminum etch rate in 4.5 % ammonium fluoride is five times lower than that of 5 % HF [28, 29]. It is very important because aluminum is usually used as an interconnect layer in sensors .
The possibilities of usage of NH4F in the MACE process are shown in , where n-type Si wafers were covered with sparse Ag particles and then etched in solutions with different NH4F concentrations. Examination by scanning electron microscope (SEM) shows that the etching of the smooth surface of n-Si (100) in 1.0 M NH4F + 5.0 M H2O2 for 1 h is leading to the formation of a PSi-like surface, where the pores were 50–150 nm in diameter and 200–300 nm in depth. In contrast, only a few shallow pores on the Si (100) surface could be formed after the etching conducted in 11.0 M NH4F + 5.0 M H2O2 for 1 h . In , the Si (100) surfaces, covered with sparse Ag particles, were put in 1.0 M NH4F + 5.0 M H2O2 to investigate their dark etching. It has been shown, that the morphology on the surface etched for 1 h revealed a sparse distribution of nanopores (10~40 nm in diameter) according to the locations of Ag particles. However, it exhibited porous surface consisting of micropores (1.5~3.1 μm in diameter with 15~20 μm in depth) where nanopores (100~150 nm in diameter) were embedded inside for the etching duration prolonged for 5 h. In ref. , it has been shown that the replacement of HF on the NH4F aqueous solution in the first MACE step, and also the usage of NH4F solution for subsequent deposition of silver particles on SiNW’s sidewall, leads to a good coating of SiNWs without formation of silver dendrites and etching pits. Such silver-coated SiNWs are proposed for surface-enhanced Raman scattering application . It was also showed that additional etching of SiNWs in NH4F leads to their surface coverage mainly with Si-(O−) x species (x = 1–3) . This, in its turn, leads to the greater stability of the samples, which is important for creating SiNW-based sensors .
In this study, SiNW arrays were prepared by MACE method, where HF is changed on NH4F in both etching steps: the decoration of the c-Si layer with Ag nanoparticles was done by using of 0.02 M of AgNO3 and 5 M of NH4F, and the etching was done in the solution containing 5 M of NH4F and 30 % of H2O2. The structure and optical properties (total reflectance, Raman scattering, and PL) of SiNWs are investigated in detail.
where ions F− and H+ were obtained not from the dissociation of HF as in the standard MACE method but from the dissociation of NH4F and H2SO4. Ag was a catalyst.
The structure properties of SiNWs were investigated by using a SEM of Lyra3 Tescan and a TEM of LEO912 AB Omega. The total reflectance spectra in the region from 250 to 1500 nm were studied with a Perkin Elmer Lambda 950 spectrometer equipped with an integrating sphere. The interband PL and Raman spectra under excitation with a cw Nd:YAG laser at 1.064 μm (excitation intensity ~100 mW; spot size ~2 mm) were measured in a backscattering geometry with a Fourier transform infrared (FTIR) spectrometer of Bruker IFS 66v/S equipped with a FRA-106 unit. PL of SiNWs in the spectral region of 500–1100 nm under excitation with ultraviolet (UV) radiation of an N2 laser (wavelength 337 nm, pulse duration 10 ns, repetition rate 100 Hz) was detected by using a grating spectrometer (MS 750, SOLAR TII) equipped with a CCD unit. All measurements were carried out at room temperature in air.
Figure 1b shows a TEM micrograph of a single SiNW. The diameter of the SiNW is about 80 nm, and it is nearly constant through the whole SiNW length. The sidewall surface of the SiNW is porous and contains silicon nanocrystals with the diameter of a few nanometers. Thus, SiNWs are structured as a single-crystal core that replicates the crystallographic orientation of the substrate and are covered by a thin (<10 nm) nanostructured layer. The same structure of SiNWs was observed for SiNWs fabricated on the lightly doped (10 Ω cm) substrate by standard MACE method .
A typical large-scale cross-sectional SEM micrograph of a sample with SiNWs is shown in Fig. 1c. One can see that SiNWs look like quasi-ordered arrays with preferential orientation along the  crystallographic direction. The length of SiNW arrays is about 2 μm. From the SEM micrograph (view from above) is seen the high density of SiNW arrays (Fig. 1d).
where hv PL—PL peak position (eV), E g —band gap of c-Si (1.12 eV), and d—nanocrystal size (nm). With the photon energy of 1.65 eV, the size of nanocrystals was about 4 nm. Same nanocrystals were observed on nanowire sidewalls in [18, 24]. The presence of the PL in the spectral region of 500–1100 nm will allow the use of SiNWs as luminescent labels for living cells as was shown for SiNWs fabricated by the standard MACE method .
Total reflectance, interband PL, Raman scattering, and PL in the spectral region of 500–1100 nm were investigated. SiNWs exhibit a strong decrease of the total reflectance to 5–15 % in the spectral region λ < 1 μm in comparison to the c-Si substrate. The PL and Raman intensities increase strongly for the SiNWs in comparison with the corresponding value of the c-Si substrate. The nanocrystal size at nanowire sidewalls was estimated from the spectral position of the PL and was about 4 nm. It was shown that optical properties of SiNWs formed by MACE using NH4F were not much different from optical properties of SiNWs formed by the standard MACE technique with HF. It gives an opportunity to obtain high-quality SiNWs for various applications in photonics, photovoltaics, and sensorics using environment-friendly chemistry.
c-Si, crystalline silicon; FTIR, Fourier transform infrared; MACE, metal-assisted chemical etching; PL, photoluminescence; PSi, porous silicon; SEM, scanning electron microscope; SiNWs, silicon nanowires; TEM, transmission electron microscope; UV, ultraviolet
The authors are grateful to V.Yu. Timoshenko for the idea of this work and helpful discussions, to A.A. Eliseev for the assistance in optical measurements, and to S.S. Abramchuk for TEM measurements. This work was partially supported by the Russian Science Foundation (Grant No. 16-13-10145) and German Federal Ministry of Education and Research (Grant No. 01DS14017) (Baltic Sea Research Network “NanoPhoto”).
KAG and AAZ performed the optical measurements and data analysis. LAO performed the SiNW fabrication. AS performed the SEM measurements. KAG, LAO, and VS performed the general data analysis and discussion of the obtained data. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Yang P, Yan R, Fardy M (2010) Semiconductor nanowire: what’s next? Nano Lett 10:1529–1536View ArticleGoogle Scholar
- Föll H, Hartz H, Ossei-Wusu E, Carstensen J, Riemenschneider O (2010) Si nanowire arrays as anodes in Li ion batteries. Phys Status Solidi RRL 4(1,2):4–6View ArticleGoogle Scholar
- Bronstrup G, Jahr N, Leiterer C, Csaki A, Fritzsche W, Christiansen S (2010) Optical properties of individual silicon nanowires for photonic devices. ACS Nano 4(12):7113–7122View ArticleGoogle Scholar
- Kelzenberg MD, Turner-Evans DB, Kayes BM, Filler MA, Putnam MC, Lewis NS, Atwater HA (2008) Photovoltaic measurements in single-nanowire silicon solar cells. Nano Lett 8:710–714View ArticleGoogle Scholar
- Sivakov V, Andrä G, Gawlik A, Berger A, Plentz J, Falk F, Christiansen SH (2009) Silicon nanowire-based solar cells on glass: synthesis, optical properties, and cell parameters. Nano Lett 9:1549–1554View ArticleGoogle Scholar
- Cui Y, Wei Q, Park H, Lieber CM (2001) Nanowire nanosensors for highly sensitive and selective detection of biological and chemical species. Science 293:1289–1292View ArticleGoogle Scholar
- Wang X, Ozkan CS (2008) Multisegment nanowire sensors for the detection of DNA molecules. Nano Lett 8(2):398–404View ArticleGoogle Scholar
- Cao A, Sudhölter EJ, de Smet LC (2015) Silicon nanowire‐based devices for gas-phase sensing. Sensors 14:245–271View ArticleGoogle Scholar
- Wagner RS, Ellis WC (1964) Vapor–liquid–solid mechanism of single crystal growth. Appl Phys Lett 4:89–90View ArticleGoogle Scholar
- Li X, Bohn PW (2000) Metal-assisted chemical etching in HF/H2O2 produces porous silicon. Appl Phys Lett 77(16):2572–2574View ArticleGoogle Scholar
- Chattopadhyay S, Li X, Bohn PW (2002) In-plane control of morphology and tunable photoluminescence in porous silicon produced by metal-assisted electroless chemical etching. J Appl Phys 91(9):6134–6140View ArticleGoogle Scholar
- Dawood MK, Tripathy S, Dolmanan SB, Ng TH, Tan H, Lam J (2012) Influence of catalytic gold and silver metal nanoparticles on structural, optical, and vibrational properties of silicon nanowires synthesized by metal-assisted chemical etching. J Appl Phys 112:073509View ArticleGoogle Scholar
- Sivakov VA, Bronstrup G, Pecz B, Berger A, Radnoczi GZ, Krause M, Christiansen SH (2010) Realization of vertical and zigzag single crystalline silicon nanowire architectures. J Phys Chem C 114:3798–3803View ArticleGoogle Scholar
- Bai F, Li M, Huang R, Song D, Jiang B, Li Y (2012) Template-free fabrication of silicon micropillar/nanowire composite structure by one-step etching. Nanosc Res Lett 7:557View ArticleGoogle Scholar
- Nahidi M, Kolasinski KW (2006) Effects of stain etchant composition on the photoluminescence and morphology of porous silicon. J Electrochem Soc 153:C19–C26View ArticleGoogle Scholar
- Sivakov VA, Voigt F, Berger A, Bauer G, Christiansen SH (2010) Roughness of silicon nanowire sidewalls and room temperature photoluminescence. Phys Ref B 82(12):125446View ArticleGoogle Scholar
- Osminkina LA, Gonchar KA, Marshov VS, Bunkov KV, Petrov DV, Golovan LA, Sivakov VA, Timoshenko VY (2012) Optical properties of silicon nanowire arrays formed by metal-assisted chemical etching: evidences for light localization effect. Nanosc Res Lett 7:524View ArticleGoogle Scholar
- Gonchar KA, Osminkina LA, Galkin RA, Gongalsky MB, Marshov VS, Timoshenko VY, Kulmas MN, Solovyev VV, Kudryavtsev AA, Sivakov VA (2012) Growth, structure and optical properties of silicon nanowires formed by metal-assisted chemical etching. J Nanoelectr Optoelectr 7(6):602–606View ArticleGoogle Scholar
- Gonchar KA, Golovan LA, Timoshenko VY, Sivakov VA, Christiansen S (2010) Effects of light localization in photoluminescence and Raman scattering in silicon nanostructures. Bull Russ Acad Sci Phys 74(12):1712–1714View ArticleGoogle Scholar
- Timoshenko VY, Gonchar KA, Golovan LA, Efimova AI, Sivakov VA, Dellith A, Christiansen SH (2011) Photoluminescence and Raman scattering in arrays of silicon nanowires. J Nanoelectr Optoelectr 6(4):519–524View ArticleGoogle Scholar
- Gonchar KA, Osminkina LA, Sivakov V, Lysenko V, Timoshenko VY (2014) Optical properties of nanowire structures produced by the metal-assisted chemical etching of lightly doped silicon crystal wafers. Semiconductors 48(12):1613–1618View ArticleGoogle Scholar
- Golovan LA, Gonchar KA, Osminkina LA, Timoshenko VY, Petrov GI, Yakovlev VV (2012) Coherent anti-Stokes Raman scattering in silicon nanowire ensembles. Laser Phys Lett 9:145–150View ArticleGoogle Scholar
- Zabotnov SV, Kholodov MM, Georgobiani VA, Presnov DE, Golovan LA, Kashkarov PK (2016) Photon lifetime correlated increase of Raman scattering and third-harmonic generation in silicon nanowire arrays. Laser Phys Lett 13:035902View ArticleGoogle Scholar
- Georgobiani VA, Gonchar KA, Osminkina LA, Timoshenko VY (2015) Structural and photoluminescent properties of nanowires formed by the metal-assisted chemical etching of monocrystalline silicon with different doping level. Semiconductors 49(8):1025–1029View ArticleGoogle Scholar
- Bertolini JC (1992) Hydrofluoric acid: a review of toxicity. J Emerg Med 10(2):163–168View ArticleGoogle Scholar
- Judge JS (1971) A study of the dissolution of SiO2 in acidic fluoride solutions. J Electrochem Soc 118(11):1772–1775View ArticleGoogle Scholar
- Dittrich T, Rauscher S, Timoshenko VY, Rappich J, Sieber I, Flietner H, Lewerenz HJ (1995) Ultrathin luminescent nanoporous silicon on n-Si: pH dependent preparation in aqueous NH4F solutions. Appl Phys Lett 67(8):1134–1136View ArticleGoogle Scholar
- Kuhl M, O’Halloran GM, Gennissen PTJ, French PJ (1998) Formation of porous silicon using an ammonium fluoride based electrolyte for application as a sacrificial layer. J Micromech Microeng 8(4):317–322View ArticleGoogle Scholar
- Ohji H, French PJ (1999) Single step electrochemical etching in ammonium fluoride. Sens Actuat A Phys 74(1–3):109–112View ArticleGoogle Scholar
- Chuang CL, Lin JC, Chao KH, Lin CC, Lerondel G (2012) On wet etching of n-Si (100) coated with sparse Ag-particles in aqueous NH4F with the aid of H2O2. J Electrochem Sci 7(4):2947–2964Google Scholar
- Lin JC, Chuang CL, Lin CC, Lerondel G (2012) Development of micro-pores including nano-pores on n-Si (100) coated with sparse Ag under dark etching in 1.0 M NH4F containing 5.0 M H2O2. J Electrochem Sci 7(8):6846–6858Google Scholar
- Sun X, Lin L, Li Z, Zhang Z, Feng J (2009) Fabrication of silver-coated silicon nanowire arrays for surface-enhanced Raman scattering by galvanic displacement processes. Appl Surf Sc 256:916–920View ArticleGoogle Scholar
- Chen WW, Sun XH, Wang SD, Lee ST, Teo BK (2005) Etching behavior of silicon nanowires with HF and NH4F and surface characterization by attenuated total reflection Fourier transform infrared spectroscopy: similarities and differences between one-dimensional and two-dimensional silicon surfaces. J Phys Chem B 109(21):10871–10879View ArticleGoogle Scholar
- Masood MN, Carlen ET, van den Berg A (2014) All-(111) surface silicon nanowire field effect transistor devices: effects of surface preparations. Mat Sci Semicond Process 27:758–764View ArticleGoogle Scholar
- Zhang M-L, Peng K-Q, Fan X, Jie J-S, Zhang R-Q, Lee S-T, Wong N-B (2008) Preparation of large-area uniform silicon nanowires arrays through metal-assisted chemical etching. J Phys Chem C 112(12):4444–4450View ArticleGoogle Scholar
- Ledoux G, Guillois O, Porterat D, Reynaud C, Huisken F, Kohn B, Paillard V (2000) Photoluminescence properties of silicon nanocrystals as a function of their size. Phys Rev B 62(23):15942View ArticleGoogle Scholar